# Electrospun Nanofibers for Integrated Sensing, Storage, and Computing Applications
## 3 Electrospun Nanofibers in Transistors: Computation and Multifunctional Electronics
### Typical Applications of Nanofiber-Based Transistors
\begin{table}
\begin{tabular}{c c c c c c c} \hline \hline
**Year** & **Nanofiber Material** & \
\begin{tabular}{c} **Mobility** \\ **(\(\mu\), cm\({}^{2}\) V\({}^{-1}\) s\({}^{-1}\))** \\ \end{tabular} &
\begin{tabular}{c} **I\({}_{\text{on}}\)/I\({}_{\text{off}}\)** \\ \end{tabular} & **Characteristics** & **Applications** & **References** \\ \hline
2011 & PANi(p-type) & \(2\times 10^{-3}\) & & Single nanofiber &
\begin{tabular}{c} Gas sensor with \\ tunable \\ sensitivity \\ \end{tabular} & [80] \\ \hline
2011 & Au-doped PANi & 11.6 & & & [65] \\ \hline
2012 & P(NDI2 OD-T2)/PEO & 0.1 & & Single fiber, Stable & [86] \\ \hline
2012 & GZO & \(10^{4}\) & &
\begin{tabular}{c} Gas sensing \\ including \\ humidity \\ \end{tabular} & [81] \\ \hline
2013 & ZnO & \(4.6\times 10^{-3}\) & &
\begin{tabular}{c} Different calcined \\ atmosphere \\ \end{tabular} & [87] \\ \hline
2013 & P3 HT/PSA & \(3.21\times 10^{-2}\) & \(10^{4}\) & Excellent air resistive ability & & [69] \\ \hline
2014 & LiNiO & \(3.3\times 10^{-4}\) & & Transparent & [88] \\ \hline
2014 & P3 DT:P3 HT & \(5.0\times 10^{-3}\) & & High bending stability & & [89] \\ \hline
2016 & ZnO & 0.018 & \(10^{3}\) & Aligned & Photoconductivity & [90] \\ \hline
2016 & PQT-12/PEO & \(1.18\times 10^{-3}\) & \(1.86\times 10^{3}\) & \
\begin{tabular}{c} Flexible, highly stable under \\ extreme bending conditions \\ \end{tabular} &
\begin{tabular}{c} Real-time \\ photosensing \\ \end{tabular} & [66] \\ \hline
2016 & MCNFs & &
\begin{tabular}{c} High sensitivity, specificity \\ and stability \\ \end{tabular} & BPA dection & [83] \\ \hline
2016 & AZO & \(3.3\times 10^{-3}\) & \(10^{3}\) & & [91] \\ \hline
2017 & PEDOT:PSS(p-type) & 5.5 & 730 & & [92] \\ \hline
2017 & CuO(p-type) & 3.5 & \(3\times 10^{5}\) & \
\begin{tabular}{c} Low operating voltage, fast \\ switching speed \\ \end{tabular} &
\begin{tabular}{c} Driving unit for \\ LED \\ \end{tabular} & [93] \\ \hline
2017 & PS/DPP & 0.22 & \(10^{3}\) & Floating-gate transistor memory & & [94] \\ \hline
2018 & NiO(p-type) & 2.8 & \(10^{4}\) & Excellent dynamic behavior & Light-emitting & [71] \\ \hline
2018 & ZnO & 0.02 & \(10^{6}\) & Low-operating voltages & & [78] \\ \hline
2018 & ZnO & 0.17 & \(2\times 10^{7}\) & Low operating voltage &
\begin{tabular}{c} Resistor-loaded \\ inverter \\ \end{tabular} & [13] \\ \hline
2018 & InGdo & 17.4 & \(10^{8}\) & Low operating voltage &
\begin{tabular}{c} Resistor-loaded \\ inverter \\ \end{tabular} & [95] \\ \hline
2018 & Mg-doped In\({}_{2}\)O\({}_{3}\) & 5.3 & \(1.7\times 10^{5}\) & & [73] \\ \hline
2019 & Sr-doped In\({}_{2}\)O\({}_{3}\) & 4.8 & \(10^{8}\) & Enhanced stability &
\begin{tabular}{c} Resistor-loaded \\ inverters \\ \end{tabular} & [96] \\ \hline
2019 & PEDOT-PSS(p-type) & 0.5 & &
\begin{tabular}{c} Non-volatile \\ charge storage \\ \end{tabular} & [97] \\ \hline
2019 & InZnO & 5.49 & \(10^{7}\) & & [68] \\ \hline
2019 & HfInZnO & 0.06 & \(10^{5}\) & & [68] \\ \hline
2019 & TiO\({}_{2}\) & &
\begin{tabular}{c} Arranged nanofibers, Mixed \\ anatase-rutile TiO\({}_{2}\) \\ \end{tabular} & [98] \\ \hline
2019 & P3 HT & 0.357 & \(4.57\times 10^{3}\) &
\begin{tabular}{c} Hollow (Coaxial \\ electrospinningning) \\ \end{tabular} & [70] \\ \hline
2020 & In\({}_{2}\)O\({}_{3}\) & 1.27 & \(5\times 10^{7}\) &
\begin{tabular}{c} Excellent reliability and \\ reproducibility \\ \end{tabular} & [99] \\ \hline
2020 & In\({}_{2}\)O\({}_{3}\) & 1.53 & \(8\times 10^{4}\) &
\begin{tabular}{c} Nontoxic and low-temperature \\ preparation \\ \end{tabular} & [76] \\ \hline
2020 & ZnSnO & 21.58 & \(10^{8}\) & \
\begin{tabular}{c} Different annealing atmosphere \\ and temperature \\ \end{tabular} &
\begin{tabular}{c} Resistor-loaded \\ inverters \\ \end{tabular} & [74] \\ \hline
2020 & IGO & 35.1 & \(10^{7}\) & Dual-gate structure & [100] \\ \hline
2020 & InYbO & 6.18 & \(10^{7}\) &
\begin{tabular}{c} Outstanding selectivity towards \\ DMF \\ \end{tabular} & Gas sensing & [101] \\ \hline \hline \end{tabular}
\end{table} 
Table 2: _Cont._